Loading in 2 Seconds...
Loading in 2 Seconds...
Ferrous Metallurgy: The Chemistry and Structure of Iron and Steel. Pure Iron. Iron from which the residual carbon left over from smelting has been removed. In the pure state it is a very soft grey metal Of no commercial use. Wrought Iron. Has approx 0.05% carbon Used since about 2000 BC
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
0.001% to 1.5% carbon
Wide range of properties due to:
Five main constituents:
The structure of pure iron.
Has a body-centred cubic (BCC) crystal structure. It is soft and ductile and imparts these properties to the steel. Very little carbon (less than 0.01% carbon will dissolve in ferrite at room temperature). Often known as iron.
This is the structure of iron at high temperatures (over 912 deg C).
Has a face-centre cubic (FCC) crystal structure. This material is important in that it is the structure from which other structures are formed when the material cools from elevated temperatures. Often known as iron. Not present at room temperatures.
A compound of iron and carbon, iron carbide (Fe3C).
It is hard and brittle and its presence in steels causes an increase in hardness and a reduction in ductility and toughness.
A laminated structure formed of alternate layers of ferrite and cementite.
It combines the hardness and strength of cementite with the ductility of ferrite and is the key to the wide range of the properties of steels. The laminar structure also acts as a barrier to crack movement as in composites. This gives it toughness.
A very hard needle-like structure of iron and carbon.
Only formed by very rapid cooling from the austenitic structure (i.e. above upper critical temperature). Needs to be modified by tempering before acceptable properties reached.
In steels none of the carbon is present as free carbon. It is all dissolved in the iron as part of the previously described structures.
Note the small amount of pearlite in the structure
A typical application of low carbon steel in a car body.
Increasing the carbon content decreases the amount of ferrite and increases the proportion of pearlite in the structure.
Note the increased amount of pearlite compared with the 0.1% ‘dead mild’ steel
This leads to an increase in strength and hardness and a reduction in ductility.
This continues until there is 0.8% carbon at which point the structure is 100% pearlite. This is known as a eutectic structure.
As carbon content increases beyond 0.8%, no more pearlite can be formed.
The excess carbon forms cementite which is deposited in between the pearlite grains. This increases the hardness, but slightly reduces the strength. The ductility of all plain carbon steels over 0.8% carbon is very low.